Effect of Saliva Contamination on Shear Bond Strength of
Transbond XT and Assure Universal Bonding Resin to Enamel
Gholamreza Eslami Amirabadi 1, Maryam Shirazi 2, Zahra Shirazi 3.
1Assistant Professor, Department of Orthodontic, School of Dentistry, Shahed University. Tehran, Iran 2Resident, Department of Orthodontic, School of Dentistry, Shahed University. Tehran, Iran
Corresponding author: Maryam Shirazi, Resident, De-partment of Orthodontic, School of Dentistry, Shahed University. Tehran, Iran
Received: 16 Nov 2013 Accepted: 26 Feb 2014
Background and Aim:Assure universal bonding resin is a modified cement with fluoride releasing property. It is claimed to provide adequate bond strength between the bracket and enamel in wet conditions; although more studies are required in this regard. This study compared the shear bond strength of Transbond XT and Assure universal bonding resin to dry and saliva-contaminated enamel in vitro.
Materials and Methods: In this in vitro study, 60 extracted human premolars were se-lected and stainless steel brackets were bonded to enamel surfaces. Bonding of brackets to enamel surfaces was done using Assure universal bonding resin (dry condition), Trans-bond XT (dry condition) and Assure (saliva-contaminated condition). The shear Trans-bond strength of brackets to the enamel was determined by Zwick/Roell machine in three groups. Data were analyzed using one-way analysis of variance (ANOVA), and the Kruskal Wallis test.
Results: The mean shear bond strength of brackets to enamel surfaces bonded with Assure (dry condition), Transbond XT and Assure (saliva-contaminated condition) was 14.18± 4.78 MPa, 16.13±5.49 MPa and 13.32±4.74 MPa, respectively (with no significant differ ences). Non-parametric Kruskal-Wallis test found no significant differences regarding the
adhesive remnant index (ARI). (p=0.053).
Conclusion: Bonding of stainless steel brackets to enamel surfaces with Assure universal bonding resin provided adequate bond strength in dry and saliva-contaminated conditions. Thus, it may be used for bonding of orthodontic brackets to the enamel surfaces in the clinical setting.
Key Words: Shear strength, Orthodontic adhesive, Dental enamel
Journal of Islamic Dental Association of IRAN (JIDAI) Summer 2014 ;26, (3)
By the introduction of acid-etch bonding systems by Buonocore in 1995 ,direct bonding of dontic brackets to teeth was made possible; ortho-dontic treatmentwasthen simplified, gingival irrita-tion decreased, oral hygiene habits became easier, esthetic needs of the patients were better achieved and orthodontic visits decreased . Acid etc-hingcreates rough surfaces that enable microme-chanical retention; enamelcrystalsbecome
prisma-ticand adherent. However, there is still a need to improve resinsand theirresistance to saliva conta-mination during bonding to reduce the incidence of failure. 
Manufacturers have tried to increase fluoride re-lease levels from the adhesives to prevent the inci-dence of white spot lesionswhile maintaining high-bond strength values. Glass ionomer cements have been found to release fluoride in the long-term, and the amountof fluoride released from them ismore
than that of fluoride-releasing composites [3-5]. Although adequate fluorideis released from these cements, their bond strengthsare poor (2.37-5.5 MPa) [6-7]. Different combinations of glass iono-mer cements and composite resins were tried for bonding brackets to the enamel surfaces. Resin modified glass ionomer cements are similar to glass ionomer cements regarding fluoride release; however, their bond strength values havebeen re-ported to be in the range of 5.39-18.9 MPa [8-11]. Bond strength values reported for the polyacid-modified composite resins were in the range of 7.3-11.97 MPa [12-13].
Conventional composite resins need completely dry surfaces to achieve clinically acceptablebond strength values; however, complete isolation of the bonding site against moisture is not possible during bracket bonding  and salivacontamination is always probable during the process of etching the enamel surface or after using primers.  In the case of contaminated enamel surfaces prior to pri-mer application, the developed porosities following acid etching areclosed off and the enamel surface energy will be decreased.Due to impaired resin penetration anddecreased micromechanical reten-tion, substantial reductions occur in the bond strength of resin to etched enamel . To solve this problem, some moisture-resistant primers have been developed.
According to astudy byFaltermeier and colleagues in 2007, Transbond XT showed no significant dif-ference in shear bond strength underdry conditions. However, the bond strength was clinically unac-ceptable using Transbond XT after saliva and blood contamination. 
Saliva contamination control anduse of materials that form proper bondsin the presence of saliva are needed. Also, with the introduction of lingual brackets, we need products that release fluoride to reduce white spot lesions.
Assure Universal Bonding Resin is a new system with fluoride releasing properties. Assure hydro-philic resin system (Reliance, Itasca, III) was ex-amined under saliva-contaminated conditions and bond strength values were found to be clinically acceptable. [14, 15]
The currentstudy compared the bond strength of Transbond XT (3M Unitek), and Assure Universal
Bonding Resin (Reliance orthodontic products, Itasca, IL) to dry and saliva-contaminated enamel.
Materials and Methods
Sixty human premolar teeth without carious le-sions, fracture, crack or attrition were collected and stored in distilled water untilthe experimentation. They were randomly allocated tothree equal groups and their buccal crown surfaces were polished with pumice paste for 15 seconds, rinsed and dried. Stainless steel metal premolar brackets were bonded to the teeth with different adhesives. Stainless steel brackets (AO, American Orthodon-tics) (12.68 mm2) were used in this study. They
were bonded to the enamel surfaces of the teeth with light-cured Transbond XT (3M) composite in the control specimens. In this group, the buccal enamel surfaces wereetched with 37% phosphoric acid for 30 seconds, rinsed for 20 seconds, and dried with oil-free air until the enamel became white. Transbond XT primer was applied to the etched surface in a thin film and Transbond XT composite was applied to the bracket base. The bracket was then positioned exactly on the tooth and compressed to expel the excess adhesive. The specimens were cured for onesecond to obtain adequate appearance. Then, additional adhesives were removed from around the brackets’ base fol-lowed by another round of light curing for 10 seconds. All these were done according to the manufacturer’s directions.
In the first experimental group, Assure Universal Bonding Resin (Reliance orthodontic products, Itasca, IL) was used. All etching, rinsing and dry-ing procedures were done accorddry-ing to Transbond XT protocol. Assure sealant was appliedin two-coats tothe buccal crown surface, left for 10 seconds, and dried slowly. Assure adhesive and Transbond XT composite wereapplied to the bracket base, and the bracket was positioned exact-ly on the tooth and compressed to expel the excess adhesive. The specimens were cured for onesecond to obtain adequate appearance. Then, excess adhe-sives were removed from around the brackets’ base followed by another round of light curing for 10 seconds.
In the secondexperimental group, all etching, rins-ing and dryrins-ing procedures were done accordrins-ing to Transbond XT protocol; however, before sealant
application, a thin layer of natural saliva was ap-plied to the enamel surface. The saliva was col-lected by the operator after teeth washing and not eating any food for onehour. The brackets were bonded similar to the previous group.
After bonding, all specimens were immersed in chloramine T solution for 24 hours at 37°C fol-lowed by storage in an incubator for oneweek at 37°C temperature. The specimens were thermo-cycled at 5°C-50°C for 1000 cycles (each cycle for 30 seconds). Each specimen was then mounted in a custom device by means of 17×25 wire. Shear loads wereapplied to the specimens at a crosshead speed of 1mm/min and 0.5 N preload force by means of Zwick machine (Zwick Roell, Germany) until bracket debonding occurred. The debonding force was recorded. Shear bond strength forces were calculated by testXpert V11.0 (Zwick Roell, Germany) software inMegapascals by dividing force (N) to bracket base area (mm2).
The debonded enamel surfaces were examined by a stereomicroscope at10× magnification and the residual adhesive remaining on the teeth was scored from 0 to 5using the adhesive remnant in-dex (ARI):
Scale 5: Adhesive and resin remained on 100% of the bracket surface
Scale 4: Adhesive and resin remained on 75%-100% of the bracket surface
Scale 3: Adhesive and resin remained on 50%-75% of the bracket surface
Scale 2: Adhesive and resin remained on 25%-50% of the bracket surface
Scale 1: Adhesive and resin remained on less than 25% ofthe bracket surface
Scale 0: No adhesive and resin remained on the bracket surface .
The shear bond strength values were analyzedby one-way ANOVA and the Kruskal Wallis test was used to assess significant differences in ARI.
The shear bond strength of brackets to the enamel surfaces was16.13±5.49 MPa (range 7.66-27.32 MPa) when bonded with Transbond XT; these val-ues were 14.18±4.78 MPa (range 7.54-25.82 MPa) for the specimens bonded with Assure Universal Bonding Resin and 13.32±4.74 MPa (range 5.6-26.9 MPa) for those bonded with Assure Universal
Bonding Resin in the saliva-contaminated enamel surfaces. One-way ANOVA showed no significant differences regarding the shear bond strength of the brackets to the teeth using Transbond XT light-cured composite, Assure and Assure in the saliva-contaminated enamel (p=0.2) (Table 1).
Table 1: Minimum, maximum, mean and standard deviation of the adhesive bond strength tostainless steel
brackets using Transbond XT and Assure (dry and wet enamel)
A indicates lack of a significant difference (P>0.05)
Different valuesof ARI using Assure, Transbond XT and Assure in saliva contaminatedgroups are presented in Table 2. Non-parametric Kruskal-Wallis test showed no significant differences in ARI among groups (p=0.053). ARI was 2 in As-sure dry enamel group, 4 in the wet enamel group and 3in the Transbond XT group. InAssureon dry enamel and Transbond XT groups, the failure rate between the bracket - adhesive and enamel - adhe-sive wasrelatively equal. In the group of Assure on wet enamel, higherfailure rate between the enamel - adhesive was noted.
As seen in Figures 1 and 2, the enamel surface under the bracket in Assure dry enamel and Transbond XT was the same. But in Assure wet enamel group a rough surface with circular holes that are likely to be related to saliva trapped in the holes, can be seen.
One of the main causes of bracket bond failure is contamination during the bonding process. It has been found that the presence of water [19, 20] or saliva [19, 21-22] can decrease the bond strength in orthodontic resin bonding systems. In the cur-rentstudy, the shear bond strengths of stainless steel brackets to the enamel bonded with Trans-bond XT and Assure in dry conditions were
16.13±5.49 MPa and 14.18±4.78 MPa, respective- ly; while the bond strength decreased to
Table 2: Frequency of different values of ARI using Transbond XT and Assure (dry and wet enamel)
Figure 1: From left to right, enamel surface under orthodontic bracket respectively: Transbond XT, Assure on wet enamel,
Assure on dry enamel. Magnification 500X (The first umn),2000X(the second column),10,000X(the third col-umn),20,000X(the fourth column). Trans bond XTgroup has a
smooth surface;in Assure on wet enamelgroup, surface is un-even and many round holes can be seen.
13.32±4.74 MPa in the saliva-contaminated tee-thusing Assure system although with no significant difference. Therefore, saliva contamination did not cause significant decreases in the shear bond strength of brackets to enamel surfaces. In other
words, using polyacidresin-modified composite resin (Assure Universal Bonding Resin)
Figure 2: From left to right: Trans bond XT, Assure on wet enamel, Assure on dry enamel, enamel interface with orthodontic bracket, respectively. B=bracket, IF=interface,
underdry and saliva-contaminated conditions did not lead toobvious changes in the shear bond strength of brackets to the enamel surfaces of the-teeth. It seems that Assure hydrophilic primer isa-ble to tolerate saliva contamination of etched ena-mel. As suggested by the manufacturer, Assure universal bonding agent with the fluoride-releasing potential can bond to normal, atypical, dry, or slightly contaminated enamel. Furthermore, it can
-5.00 4.00 3.00 2.00 1.00 .00
4 6 8 1 0 Count
20/0% 30/0% 40/0% 5/0% 0%
5 7 6 1 1 Count
25/0% 35/0% 30/0% 5/0% 5/0% %within group
10 4 3 0 1 Count
50/0% 20/0% 15/0% 0%
5/0% %within group
19 17 17 2
31/7% 28/3% 28/3% 3/3% 3/3% %within group
be used with any light- or chemical-curing sys-tems.
Other studies regarding the bond strength of bond-ing systems underthe saliva-contaminated condi-tions have reported controversial findings; some have noted an increase in bond strength values [23, 24], whileothers found no significant changes  or a significant decrease.  Differences in the experimental protocols, use of artificial or human saliva as well as the quantity of the applied saliva can explainsuchdifferent results. In addition, the composition of saliva can be different based onthe conditions under which it was produced.
The other possible reason can be the presence of water in the composition of hydrophilic primers. All these can affect bond strength of the brackets to the enamel.
Rix et al. (2001) reported higher bond strength values for Transbond XT specimens; although adequate bond strength of brackets to the enamel was noted in their study when bonding with Assure indry and wet conditions (10.74 MPa and 10.99 MPa); similar to our findings . They showed that bond strength of the Assure adhesive was not significantly affected by dry orwet conditions. In contrast to our results, Oztoprak et al. (2007) showed that saliva (10.66 MPa versus 16.4 MPa) and blood contamination (6.83 MPa versus 16.4 MPa) significantly decreased bond strength values compared to dry conditions . Furthermore, Webster et al. (2001) reported the Assure system to show more tolerance against saliva contamination similar to our study results . Again, Schane-weldt et al. (2002) concluded that the bond strength of Assure and MIP primers are not af-fected by saliva contamination . Similarly, Nemeth et al. (2006) reported that bond strength of Assure to enamel contaminated with saliva is bet-ter than other mabet-terials . It seems that bonding to bothdry and wet enamel surfaces depends on the material itself and sufficientbond strengths to wet and saliva-contaminated enamel surfaces can be achieved using appropriate materials.
The reported bond strength in different studies maybe related to the factors such as thermocycling tests, bond strength testing machines, direction of the force applied to debond the brackets, the cross-head speed, bracket type, standardization of mois-ture application, quality and quantity of the
prod-ucts as well as thediversity in the used materials and methods .
In routine orthodontic practice, achievement of adequate bond strength for safe debonding is more favorable than obtaining the maximum possible bond strength . Therefore, ARI scores are used in different studies to determine the site of bond failure between the enamel, the adhesive, and the bracket base via observation of the remaining composite on the enamel surfaces. In orthodontic bond strength examinations, cohesive failures in the composite (ARI score 3) indicate the internal strength of the composite rather than the adhesion to the surface under investigation 
In the currentstudy, the frequency of ARI scores of 2 (40%) and 3 (30%) washigher for Assure compo-site system; ARI scores of 3 (25%) and 2 (30%) were found frequently in Transbond XT and scores of 4 (50%) and 3 (20%) were higher for Assure in the saliva-contaminated conditions. When bonding to wet enamel, higher scores of ARI were recorded suggesting unfavorable bonding atthe bracket-adhesive interface. According to the SEM results, the mentioned finding is likely due to the accumu-lation of saliva in the area and creation ofbubbles under the brackets reducing the enamel - bracket bond strength and increasing failures in this area.
Bonding stainless steel brackets to the enamel sur-faces with Assure Universal Bonding Resin pro-duced adequate bond strength in bothdry and sali-va-contaminated conditions. Thus, it can be used for bonding orthodontic brackets to the enamel surface in the clinical setting.
1. Buonocore MG. A simple method of increasing the adhesion of acrylic filling materials to enamel surfaces. J Dent Res. 1955 Dec;34(6):849-53. 2. Bishara SE, Olsen ME, Damon P, Jakobson JR. Evaluation of a new light-cured orthodontic bond-ing adhesive. Am J Orthod Dentofacial Orthop. 1998. Jul;114(1):80-7.
3. Chadwick SM, Gordon PHH. An investigation into the fluoride release of a variety of orthodontic bonding agents. Br J Orthod. 1995 Aug;22(3):279-81.
4. Forsten L. Short- and long-term fluoride release from glass ionomers and other fluoride-containing filling materials in vitro. Scand J Dent Res. 1990 Apr;98(2):179-85.
5. Takahashi K, Emilson CG, Birkhed D. Fluoride release in vitro from various glass ionomer ce-ments and resin composites after exposure to NaF solutions. Dent Mater. 1993 Nov;9(6):350-4. 6. Wiltshire WA. Shear bond strengths of a glass ionomer for direct bonding in orthodontics. Am J Orthod Dentofacial Orthop. 1994 Aug;106(2):127-30.
7. Fajen VB, Duncan MG, Nanda RS, Currier GF, Angolkar PV. An in vitro evaluation of bond strength of three glass ionomer cements. Am J Or-thod Dentofacial Orthop. 1990 Apr; 97(4):316-22. 8. Ewoldsen N, Beatty MW, Erickson L, Feely D. Effects of enamel conditioning on bond strength with a restorative light-cured glass ionomer. J Clin Orthod. 1995 Oct;29(10):621-4.
9. Meehan PM, Foley TF, Mamandras AH. A comparison of the shear bond strengths of two glass ionomer cements. Am J Orthod Dentofacial Orthop. 1999 Feb;115(2):125-32.
10. Lippitz SJ, Staley RN, Jakobsen JR. In vitro study of 24-hour and 30-day shear bond strengths of three resin-glass ionomer cements used to bond orthodontic brackets. Am J Orthod Dentofacial Orthop. 1998 Jun;113(6):620-4.
11.CacciafestaV, Jost-Brinkmann PG, Su Benberger U, Miethke RR. Effects of saliva and water contamination on the enamel shear bond strength of a light-cured glass ionomer cement. Am J Orthod Dentofacial Orthop. 1998 Apr; 113(4):402-7.
12. Rock WP, Abdullah MSB. Shear bond strengths produced by composite and compomer light cured orthodontic adhesives. J Dent. 1997 May-Jul;25(3-4):243-9.
13. Ashcraft DB, Staley RN, Jakobsen JR. Fluoride release and shear bond strengths of three light-cured glass ionomer cements. Am J Orthod Den-tofacial Orthop. 1997 Mar; 111(3):260-5.
14. Zeppieri IL, Chung C-H, Mante FK. Effect of saliva on shear bond strength of an orthodontic adhesive used with moisture-insensitive and self-etching primers. Am J Orthod Dentofacial Orthop. 2003 Oct;124(4):414-9.
15. Schaneveldt S, Foley TF. Bond strength com-parison of moisture-insensitive primers. Am J Or-thod Dentofacial Orthop. 2002 Sept;122(3):267-73. 16. Rajapodal R, Padmanabhan S, Gnanamani J. A comparison of shear bond strength and debonding characteristics of conventional, moisture-insensitive and self-etching primers in vitro. Angle Orthod. 2004 Apr;74(2):264-8.
17.Faltermeier A, Behr M, Rosentritt M, Reicheneder C. An in vitro comparative assessment of different enamel contaminants during bracket bonding. Eur J Orthod. 2007 Dec; 29(6):559.
18. Turgut M, Attar N, Korkmaz Y, Gokcelik A. Comparison of shear bond strengths of orthodontic brackets bonded with flowable composites. Dent Mater J. 2011 Jan;30(1):66-71.
19. Cacciafesta V, Sfondrini M, DeAngelis M, Scribante A, Klersy C. Effect of water and saliva contamination on shear bond strength of brackets bonded with conventional, hydrophilic, and self-etching primers. Am J Orthod Dentofacial Orthop. 2003 Jun; 123(6):633-40.
20. Kula KS, Nash TD, Purk JH. Shear-peel bond strength of orthodontic primers in wet conditions. Orthod Craniofacial Res. 2003 May;6(2):96-100. 21.Nemeth BR, Witahire WA, Levete CL. Shear/peel bond strength of orthodontic attachments to moist and dry enamel. Am J Orthod Dentofacial Orthop. 2006 Mar;129(3):396-401.
22. Sirirungrojying S, Saito K, Hayakawa T, Kasai K. Efficacy of using self-etching primer with a 4-Meta/MMA-TBB resin cement in bonding ortho-dontic brackets to human enamel and effect of sa-liva contamination on shear bond strength. Angle Orthod. 2004 Apr;74(2):251-8.
23. Oztoprak MO, Isik F, Sayinsu K, Arun T, Ay-demir B. Effect of blood and saliva contamination on shear bond strength of brackets bonded with 4 adhesives. Am J Othod Dentofacial Orthop. 2007 Feb;131(2):238-42.
24. Sayinsu K, Isik F, Sezen S, Aydemir B. Effect of blood and saliva contamination on bond strength of brackets bonded with a protective liquid polish and light-cure adhesive. Am J Orthod Dentofacial Orthop. 2007 Mar;131(3):391-4.
25. Cacciafesta V, Sfondrini M, DeAngelis M, Scribante A, Klersy C. Effect of water and saliva contamination on shear bond strength of brackets bonded with conventional, hydrophilic, and
etching primers. Am J Orthod Dentofacial Orthop. 2003 Jun; 123(6):633-40.
26. Turk T, Elekdag-Turk S, Isci D, Cakmak F, Ozkalayci N. Saliva contamination effect on shear bond strength of self-etching primer with different debond times. Angle Orthod. 2007 Jan :77:901-906.
27. Rix D, Foley TF, Mamandras A. Comparison of bond strength of three adhesives: Composite resin, hybrid GIC, and glass-filled GIC. Am J Or-thod Dentofacial Orthop. 2001 Jan; 119(1):36-42. 28. Webster MJI, Nanda RS, Duncanson MGJR, Khajotia SS, Sinha PK. The effect of saliva on shear bond strengths of hydrophilic bonding sys-tems. Am J Orthod Dentofacial Orthop. 2001 Jan; 119(1):54-8.
29. Santos BM, Pithon MM, de Oliverira Ruellas AC, Sant’Anna EF. Shear bond strength of brack-ets bonded with hydrophilic and hydrophobic bond systems under contamination. Angle Orthod. 2010 Sept;80(5):963-7.
30. Saito K, Sirirungrojying S, Meguro D, Haya-kawa T, Kasai K. Bonding durability of using self-etching primer with 4-META/MMA-TBB resin cement to bond orthodontic brackets. Angle Or-thod. 2005 Mar;75(2):260-5.
31. Zachrisson BU, Buyukyilmaz T. Surface prep-aration for orthodontic bonding to porcelain. Am J Orthod Dentofacial Orthop. 1996 Apr;109(4):420-30.